# i.introduction - arxiv

Embed Size (px)

TRANSCRIPT

Thermoelectric performance of P-N-P abrupt heterostructures

vertical to temperature gradient Bohang Nan, Guiying Xu*, Quanxin Yang and Tao Guo

Beijing Municipal Key Lab of Advanced Energy Materials and Technology, School of Materials Science and Engineering, University of Science and Technology Beijing,

Beijing 100083, China Corresponding authors: [email protected] (G. Xu)

Abstract. We present a model for P-N-P abrupt heterostructures vertical to temperature gradient to

improve the thermoelectric performance. The P-N-P heterostructure is considered as an abrupt bipolar junction transistor due to an externally applied temperature gradient paralleled to depletion layers. Taking Bi2Te3 and Bi0.5Sb1.5Te3 as N-type and P-type thermoelectric materials respectively for example, we achieve the purpose of controlling the Seebeck coefficient and the electrical conductivity independently while amplifying operation power. The calculated results show that the Seebeck coefficient can reach 3312V/K, and the ZTmax values of this model are 45 or 425, which are tens or even hundreds of times greater than those of bulk materials and films.

I. Introduction It is well known that energy issue is imperative for most countries in

the world. Many researchers have searched for novel sustainable and

renewable energy sources in order to alleviate energy consumption needs

and increase utilization efficiency. Thermoelectric materials have

attracted a lot of attention because of their reversible conversion between

heat and electricity.

Thermoelectric performance is quantified by the dimensionless

figure of merit 2 /ZT S T , where S is the Seebeck coefficient, is

the electrical conductivity, T is the absolute temperature and is the

thermal conductivity.[1] Thermal conductivity primarily includes the

lattice thermal conductivity ( L ) and the electronic thermal conductivity

( e ). , 2S is called “power factor” of the thermoelectric material.

However, these parameters are mutually influential, which makes it

difficult to enhance thermoelectric performance. Therefore, most

traditional bulk thermoelectric materials can reach max 1ZT , such as

Bi2Te3, PbTe and SiGe alloys.[2]

Generally speaking, if the commercial thermoelectric materials have

a higher ZT, their conversion efficiency would be higher.[3] And

thermoelectric materials need have ZT values greater than 3 to be

competitive with traditional mechanical equipment.[4]

In order to enhance ZT values, low-dimensional thermoelectric

materials have become the forefront of research since 1990s. Hicks and

Dresselhaus initially presented the concept that low-dimensional

materials could increase their thermoelectric performance after improving

its power factor in 1993.[5] Based on their assumptions, a max 6ZT for

the Bi2Te3 two-dimensional material was obtained. This prediction was

confirmed by many experimental data. The high ZTmax value of 2.4 in

P-type Bi2Te3/Sb2Te3 quantum-well superlattice material was prepared by

Venkatasubramanian et al.[6] Then a greatly enhanced ZTmax value of 3

was obtained in N-type PbSeTe/PbTe quantum-dot superlattice material

by Harman et al.[7] In addition, 1ZT silicon nanowires achieved by

Boukai et al were one hundred times greater than bulk silicon materials.[8]

Hinterleitner et al. prepared Fe2V0.8W0.2Al films by magnetron sputtering,

which reached a maximum ZTmax of 6 around 350-400K.[9]

These enhanced thermoelectric performances mainly originated

from two aspects: (1) the Seebeck coefficient can be improved by

introducing quantum confinement effect;[10,11] (2) the lattice thermal

conductivity can be decreased because phonons are effectively scattered

by interfaces.[12-14] However, there are some questions that hinder the

development of low-dimensional thermoelectric materials. First of all, the

improved ZT values of most low-dimensional thermoelectric materials are

derived from the reduction of the lattice thermal conductivity, rather than

the increase of power factor. Secondly, it is difficult to control S and

independently. Therefore, it is a more common choice to make the

addition of the Seebeck coefficient greater than the reduction of the

electrical conductivity.

In order to solve these questions, we present a model for the P-N-P

heterostructure, which was designed through arranging several P-N

junction thermoelectric materials in a certain structure. In fact, P-N

junctions have been studied a lot and used widely since 1950s. In the late

1990s, P-N junctions were predicted to enhance Seebeck coefficients and

ZT values of thermoelectric materials by Dashevsky,[15] Zakhidov,[16]

Ravich[17] and others. Wagner and Span proposed a new approach that

P-type material and N-type material could be directly connected without

metal electrodes. Meanwhile, a temperature gradient was applied along

this P-N junction, as shown in Figure 1.[18] The measured results

demonstrated that the efficiency of this approach is higher than traditional

P-N junctions.[19] Further research on this approach was carried out by Fu

Deyi et al. Fu Deyi theorized that this approach could increase the

Seebeck coefficient and decrease the electronic thermal conductivity due

to the effect of eddy currents in the P-N junction.[20]

Figure 1. P-N junction with applied temperature gradient

In this work, we propose a P-N-P abrupt heterostructure model

vertical to temperature gradient, and provide the detailed analysis process

along with calculated results. Here, due to the effect of temperature

gradient, the P-N-P heterostructure behaves as a bipolar junction

transistor to achieve power amplification. The collector current is

controlled by the emitter current in a bipolar transistor, while the Seebeck

coefficient is controlled by base-collector interface. The purpose of

independent control with regards to both the Seebeck coefficient and

electrical conductivity is realized. As a result, the ZTmax values can reach

tens or even hundreds of times greater than those of bulk materials and

films.

The paper is organized as follow: In Sec. II we shall describe our

model for P-N-P heterostrctures. In Sec. III we will show and discuss our

calculated results. In Sec. IV we shall conclude.

The scheme that has been adopted with respect to notation is

illustrated by the partial list of symbols shown in Table I. In addition, the

symbol μ has been employed for charge carrier mobility, D for diffusion

constant. Table I. Partial list of symbols used

Symbol meaning

Na, Nd Doping concentration in a P-type material, in a N-type material.

Ex Electric field intensity in an abrupt P-N junction.

xp, xn Depletion layer width near a P-type region, near a N-type region

Electric potential variation in an abrupt P-N junction

r Relative permittivity of the material

0 Vacuum dielectric constant

ni Intrinsic carrier concentration of the material

Vs The Seebeck voltage generated by the temperature gradient.

EC, EV Conduction band minimum of the material, valence band maximum of the material.

EFp, EFn The quasi-Fermi level in a P-type material, in a N-type material.

m* The effective mass of the material.

II. Analytical model for P-N-P heterostructures An analytical model for thermoelectric properties of P-N-P

heterostructure is presented in this section. Under the effect of

temperature gradient, P-N-P heterostructures behave as a bipolar

transistor. A general circuit diagram of a P-N-P heterostructure is shown

in Figure 2, where P-type material (at the left side of this figure) is

considered as an emitter material, N-type material is treated as a base

material, and another P-type material (at the right side of this figure) is

acts as a collector material. In addition, there are depletion layers at the

both of base-emitter interface and at the base-collector interface. The base

width is considered to be the sum of the width of both depletion layers

near N-type region. As a result, the base region can serve as an insulating

layer, in which majority carriers have been depleted. The direction of

temperature gradient is assumed to be parallel to these depletion layers.

Therefore, in the X direction, the Seebeck voltage can be produced due to

the existence of temperature gradient. Meanwhile, the Seebeck voltage

can become an external power supply in the bipolar transistor. We have

biased the emitter forward and the collector in reverse to achieve the

purpose of power amplification. We have also treated the bipolar

transistor as two coupled P-N diodes, according to the Ebers-Moll

model.[21]

In order to simplify this calculation, we have adopted several

assumptions: (1) abrupt P-N junctions; (2) Depletion layer approximation;

(3) Long-length approximation; (4) some assumptions for the bipolar

transistor.

We have divided this bipolar transistor into two coupled P-N

junctions and assumed these P-N junctions are all abrupt junctions, which

means that impurities are uniformly distributed in different regions. For

one abrupt P-N junction, doping levels in P-type material and N-type

material are kept constant when it is away from this junction and will

abruptly change at the junction interfacial region (as in Figure 3b). It is a

consensus that a dN N in the P-type region and d aN N in the N-type

region. As a result physical parameters of the abrupt P-N junction usually

vary in different regions, such as electric field intensity (as in Figure 3c)

electric potential (as in Figure 3d) and doping levels.[22]

Figure 3. (a).An abrupt P-N junction; (b). Doping levels for the abrupt junction; (c). Electric field intensity for the abrupt junction; (d). Electric potential variation for

the abrupt junction.

We have found that the electric field intensity is zero and the electric

potential variation is constant when away from the junction interfacial

region in thermal equilibrium. Therefore, we have divided this P-N

junction into three regions: P-type region, N-type region and depletion

layer, where the depletion layer has an electric potential difference and

other regions are neutral.

(2)Depletion layer approximation

If P-type material and N-type material combine to form a P-N

junction, the majority carriers of two regions will move to the opposite

area due to carrier concentration gradients that exist at the interface. It

results in a depletion layer at the interface when the equilibrium is

reached again.

To solve for the potential barrier biV across the depletion layer, we

have employed the depletion layer approximation. In this assumption,

there are no free electrons and holes in the depletion layer, only impurity

ions ( dN or aN ). Moreover, recombination is completely neglected in the

depletion layer. As a result, the potential barrier biV can be obtained by

solving Possion’s equation:[23]

2 04 / r (1)

2ln d aB bi

(2)

We have also utilized another assumption that the voltage drop will

only appear at the depletion layer if an external voltage (Vs) is applied.

Simultaneously, the potential barrier is independent of the temperature

gradient and external voltage.

Generally, there are different Fermi levels between P-type material

and N-type material. Therefore, the Fermi level can be realigned during

the process of forming a PN junction, resulting in the quasi-Fermi level.

To simplify this analysis, we have adopted the assumption that the

quasi-Fermi level is constant.[24]

In reality, minority carriers of P-type material and N-type material

need to be considered. This is because the recombination of minority

carriers and majority carriers can affect the performance of a P-N

junction. Therefore, the long-length approximation has been employed,

in which the electron and hole diffusion lengths are shorter than the

widths of P-type and N-type regions.[25] In other words, electrons and

holes are recombined completely in the neutral region. The specific

description is shown in Figure 4:

Figure 4: P-N junction in long-length approximation

The quasi-Fermi level ( FnE ) of N-type material is therefore constant

in N-type region and the depletion layer under the same temperature, and

the same applies to P-type material. The quasi-Fermi level is directly

reflected in the dependence of the carrier concentration, resulting in a

convenient calculation for the Seebeck coefficient:

5 2

B F

(3a)

sV S T (3b)

Where 1/ 2r is the phonon scattering parameter, sV is the

Seebeck voltage, and T is the temperature difference.

In this model, we have used Seebeck coefficients of bulk N-type

material and P-type material as the basis for calculating the Seebeck

voltage of the P-N junction.

(4 ) Some assumptions about the bipolar transistor

Although we have divided the bipolar transistor into two P-N

junctions during the analysis process, the expression for volt-ampere

characteristic of the bipolar transistor is still essential when calculating

the overall thermoelectric performance. The suitable expression for

volt-ampere characteristic of the bipolar transistor is not only based on

above assumptions, but also requires some further hypotheses.

In our model, the base width is very thin(around 20nm) and the

recombination of electrons and holes in the base region is neglected so

that the base current is equal to zero, which means that the emitter current

is equal to the collector current. Meanwhile, we have adopted small

injection levels. Therefore, the expression for volt-ampere characteristic

of the bipolar transistor is written as:

/ 1E BpB nB nE pE qV k T E

B nE

W L

where EJ is the emitter current density, B pB pB

k TD q

is the hole

diffusion coefficient of the base material, pB is the minority carrier

mobility of the base material, nBP is the minority carrier concentration of

the base material, BW is the base width, B nE nE

k TD q

is the electron

diffusion coefficient of the emitter material, nE is the minority carrier

mobility of the emitter material, pEN is the minority carrier

concentration of the emitter material, nE nE nEL D is the minority

carrier diffusion length of the emitter material, nE is the relaxation time

of the emitter material, and EV is the emitter voltage.

We have assumed the emitter current is equal to the collector current,

and the current density of both is the same if junction areas of the

base-emitter interface and base-collector interface are identical. Therefore,

E CJ J can be obtained.

Subsequently, the collector voltage and emitter voltage can thus be

determined. We have assumed that the emitter is forward biased and the

collector is reverse biased. In addition, the Seebeck voltage caused by the

temperature gradient is treated as an external power supply for the bipolar

transistor. Moreover, the potential barrier E biV of the base-emitter

interface and the potential barrier C biV of the base-collector interface are

independent of the external voltage. Therefore, the emitter voltage EV

and collector voltage CV can be written as:

E E bi EV V S T (5a)

C C bi CV V S T (5b)

where ES is the Seebeck coefficient of the emitter material, and CS is

the Seebeck coefficient of the collector material.

After determining EV and CV , the depletion layer width ( dCx ) across

the base-collector interface can be written as:

02 r C a

nC d a d

dC nC pCx x x (6c)

where nCx is the depletion layer width near the base region, and

pCx is the depletion layer width near the collector region. And the

depletion layer width across the base-emitter interface ( dE nE pEx x x ) can

also be obtained. Consequently, the base width in Eq.(4) is equal to

nEx + nCx .

The electrical conductivity of the bipolar transistor can be derived

from the emitter current density:

eJ E

base-emitter interface (depletion layer) as the electric field varies linearly

with distance for an abrupt P-N junction.

The Seebeck coefficient of the bipolar transistor can be obtained

based on the collector voltage:

c PNP

VS T

(8)

Finally, the power factor and ZT of the bipolar transistor can also be

obtained:

bipolar transistor can be obtained.

III. Result and Discussion

The model described in this work has been implemented using

MATLAB. Because Bi2Te3 and Sb2Te3 are widely used thermoelectric

semiconductor materials, we applied our model to a

P-Bi0.5Sb1.5Te3/N-Bi2Te3/ P-Bi0.5Sb1.5Te3 heterostructure in order to

evaluate the potentiality of this model. Table II. shows these material

parameters used in the simulation. Table II. Material parameters used for the simulation (Tc=298K Th=323.15K)

Material Parameter

Emitter (P-Bi0.5Sb1.5Te3)

Base (N-Bi2Te3)

Collector (P-Bi0.5Sb1.5Te3)

Eg(eV) 0.18[26] 0.17[27] 0.18 r 260[26] 400[28] 260 m*/m0 1.441[29] 1.4[30] 1.467[29]

n(cm2/V s) 120[31] 1200[17] 120 8000[32] \ 8000[32]

p(cm2/V s) \ 510[17] \ \ 4778.3[33] \

Dn(cm2/s) 3.3446 33.466 3.3446 222.97 \ 222.97

Dp(cm2/s) \ 14.2146 \ \ 133.18 \

doping concentrations for the emitter material, base material and collector

material according to Eq.(3a). In order to obtain the better thermoelectric

performance, we set the range of Seebeck coefficients for these materials

at 220V/K240V/K. Therefore, the scope of doping concentrations

for these materials can subsequently be determined. These results are

derived from experimental data found in previous literature.[29,30]

Figure 5. The relationship between Seebeck coefficients and doping concentrations for (a) the base material, (b) the emitter material, and (c) the collector material

We could estimate the range of doping concentrations for these

materials through calculated results. The range for base material, emitter

material, and collector material is 19 19 32.1 10 2.7 10 / cm ,

19 19 32.2 10 2.8 10 / cm and 19 19 32.2 10 2.8 10 / cm respectively.

2.1 Collector voltage

According to Eq. (5b), the collector voltage is the sum of the

potential barrier of the base-collector interface and the Seebeck voltage.

Moreover, we considered that the collector voltage is a function of the

base doping concentration and collector doping concentration based on

Eq.(2) and Eq.(3a), as shown in Figure 6.

Figure 6. Collector voltage in the P-N-P heterostructure

In order to obtain the maximum output power, the collector voltage

should be at the maximum. We can see that the maximum collector

voltage is 0.1656V when doping concentrations of the base material and

collector material are 19 32.7 10 / cm and 19 32.8 10 / cm , respectively.

Therefore, we can determine the optimal doping concentrations for the

base material and collector material. Subsequently, 11.75nCx nm can be

obtained to calculate the base width .

2.2. Emitter voltage and Emitter current density

After determining the base doping concentration, the emitter voltage

is also derived from Eq.(2), (3a) and (5a). Figure 7 shows the relationship

of the emitter voltage and the emitter doping concentration.

Figure 7. Emitter voltage in the P-N-P heterostructure

We find that the magnitude of the emitter voltage increases as the

emitter doping concentration increases. This finding indicates that the

potential barrier of the base-emitter interface is positively correlated with

the emitter doping concentration and the Seebeck voltage is relatively

small. But we can’t define the optimal doping concentration of the emitter

material just from Figure 8 as the emitter current density is a more

important parameter for the bipolar transistor. As a result, we calculated

the emitter current density based on data presented in Table II. The

relationship between the emitter current density and the emitter doping

concentration under different carrier mobility is shown in Figure 8.

Figure 8. Emitter current density in the P-N-P heterostructure

(a) 2 1 1510p cm V s for the base material, 2 1 1120n cm V s for the

emitter material (b) 2 1 14778p cm V s for the base material,

2 1 18000n cm V s for the emitter material (c) 2 1 1510p cm V s for the

base material, 2 1 18000n cm V s for the emitter material (d)

2 1 14778p cm V s for the base material, 2 1 1120n cm V s for the emitter

material

As it can be seen, there are different emitter current densities under

distinct carrier mobility and the absolute values of emitter current

densities increase with the increase of the emitter doping concentration.

In order to gain the maximum output power, we determined the emitter

current density should be the maximum and also obtained the optimal

emitter doping concentration along with the maximum emitter voltage.

Meanwhile, the depletion layer width ( nE pEx x ) across the base-emitter

interface and the base width ( nEx + nCx ) were determined.

We summarized the maximum emitter current densities under

different conditions in Table III. Table III. The maximum emitter current densities under different carrier mobility

(T=323.15K) Carrier Mobility

It is evident that the maximum emitter current densities remain

almost unchanged when the minority carrier mobility ( p) of the base

material is constant from Table III. This is because the base width is

nanoscale and the electron diffusion length of the emitter material is

micron level. Therefore, we considered that the minority carrier mobility

of the base material is the main factor affecting the maximum emitter

current densities. Moreover, the nanoscale base width results in a large

emitter current density, which increases the output power in the bipolar

transistor.

Because we selected the optimal collector voltage and the maximum

emitter current density, the optimal electrical conductivity and Seebeck

coefficient of the bipolar transistor can be obtained according to Eq.(7)

-(9b). Specific calculation results are shown in Table IV.

Table IV. Electrical conductivities, Seebeck coefficients, power factors and ZT for the P-N-P heterostructure (T=323.15K)

Case Carrier Mobility /cm2/V s

Electrical Conductivity /S/cm

Seebeck Coefficient /V/K

255.9 3312 2807.06 45

2397.7 3312 26301.2 425

256.44 3312 2813 45

2397.7 3312 26301.2 425

The electrical conductivities of all the cases are shown in Table IV.

We can find that these cases have electrical conductivities of about

255.9S/cm, 2397.7S/cm, 256.44S/cm and 2397.7S/cm, respectively. The

magnitude of electrical conductivity of all the cases change with the hole

mobility of base material (N-type Bi2Te3). Compared with N-type Bi2Te3

bulk material ( 1204.5 /S cm )[29] and film ( 2174 /S cm )[34] in previous

literature, electrical conductivities of Case I and Case III are lower than

those of the bulk material and film. Because electrical conductivities are

derived from Eq.(4) and Eq.(7), we consider that the emitter current

density is the main factor affecting electrical conductivities. We can see

that the emitter current density is related to minority carrier

concentrations at the base region and the emitter region in Eq.(4).

Therefore, possible explanation behind the low electrical conductivities

of Case I and Case III is the relatively low minority carrier concentrations

at the base-emitter interface. On the other hand, Case II and Case IV have

almost the same electrical conductivities as films. This is because the

minority carrier mobility of these two cases is larger than those of films

( 210.7 /cm Vs ) in Reference [34]. We believe that the reduction in the

carrier concentration is more than compensated for by the increase in the

carrier mobility.

The Seebeck coefficients of these cases exhibit very large absolute

values, which are 50 times greater than those of films and 15 times

greater than those of bulk materials. We believe that such a large Seebeck

coefficient may be caused by the potential barrier of the depletion layer in

the base-collector interface. In this depletion region, majority carriers can

be depleted completely and the recombination of electrons in N-type

material and holes in P-type material at the cold region under this

temperature gradient can be eliminated. Therefore, the high values of

Seebeck coefficients can be obtained.

So far, we have considered only electrical conductivities and

Seebeck coefficient since it is through these performances that our model

predicts an increase in ZT. However, ZT is also in dependence of the

thermal conductivity . If we assume that the thermal conductivity of the

bipolar transistor is equal to 2W/m K, our calculated results in Table III

imply that the bipolar transistor ZT can be up to dozens of times or even

hundreds of times greater than bulk and film values, giving values

of max 45ZT in Cases I and III and max 425ZT in Cases II and IV at

323.15K.

IV. Summary

In this paper, we present a general model for P-N-P heterostructures.

In our model, P-N-P heterostructures behave as bipolar transistors due to

the setting of temperature gradient. We take an abrupt

P-Bi0.5Sb1.5Te3/N-Bi2Te3/ P-Bi0.5Sb1.5Te3 heterostructure as example to

obtain thermoelectric performance of this model. The electrical

conductivity based on the emitter current density and the Seebeck

coefficient based on the collector voltage for the bipolar transistor were

calculated in order to control the Seebeck coefficient and the electrical

conductivity independently. The conclusion can be obtained as below.

(1) With the optimal doping concentration of 19 32.7 10 / cm ,

19 32.8 10 / cm and 19 32.8 10 / cm for the base material, emitter material and

collector material, respectively, the maximum emitter current density and

the maximum collector voltage under different carrier mobility are 1.892

×1011A/m2 or 1.769×1012A/m2 and 0.1656V. The maxZT values can reach

45 or 425 at 323.15K. Therefore, this model is a useful method to

enhance thermoelectric performances and efficiency.

(2) This P-N-P heterostructure model not only provides a completely

new perspective for research in the thermoelectric field, but also for other

energy conversion mechanisms, such as photovoltaic conversion.

Acknowledgements:

This work was financially supported by The National Key Research

and Development Program of China [Grant No. 2017YFF0204706], by

the Fundamental Research Funds for the Central Universities [Grant No.

FRF-MP-18-005, and FRF-MP-19-005].

B pE

W L

11 32.26 10 /in cm , 2112

6 3 16

, 500BW nm ,

610n s in the base , 75 10p s in the emitter, 2 122.5nBD cm s ,

2 16.5pED cm s , 18pL m ,

2112 5 3

, 8 21.44 10 /EJ A m is shown in the

literature.

We utilize Eq.(A1) to obtain the emitter current density ' EJ based on these data

and compare with EJ .

Therefore, ' 8 21.41 10 /EJ A m is obtained. And the result is very close to

EJ .

Finally, we can conclude that Eq.(4) and Eq.(A1) are all effective for calculating emitter current densities of P-N-P bipolar transistors and N-P-N bipolar transistors.

Reference: [1] G.J. Snyder, E.S. Toberer. Complex thermoelectric materials[J]. Nature Materials, 2008, 7(2):105-114. [2] J.Mao, Z.Liu, Z.Ren. Size effect in thermoelectric materials[J]. Nature, 2016, 1(1). [3] Z.G.Chen, G.Han, L.Yang, L.N.Chen, J.Zou. Nanostructured thermoelectric

materials: Current research and future challenge[J]. Progress in Natural Science Materials International, 2012(6):535-549. [4] C.J.Vineis, A.Shakouri, A.Majumdar, M.G.Kanatzidis. Nanostructured Thermoelectrics: Big Efficiency Gains from Small Features[J]. Advanced Materials, 2010, 22(36):3970-3980. [5] L.D.Hicks, M.S.Dresselhaus.Effect of quantum-well structures on the thermoelectric figure of merit[J]. Physical Review B, 1993, 47 (19):12727-12731. [6] R.Venkatasubramanian, E.Siivola, T.Colpitts, B.O’Quinn.Thin-film thermoelectric devices with high room-temperature figures of merit[J]. Nature, 2001, 413: 597-602. [7] T.C.Harman, M.P.Walsh, B.E.Laforge, G.W.Turner. Nanostructured thermoelectric materials[J]. Journal of Electronic Materials, 2005, 34(5):L19-L22. [8] A.I.Boukai, Y.Bunimovich, J.Tahir-Kheli, et al. Silicon nanowires as efficient thermoelectric materials[J]. Nature, 2008, 451(7175):168-171 [9] B.Hinterleitner B, I.Knapp, M.Poneder, et al. Thermoelectric performance of a metastable thin-film Heusler alloy[J]. Nature, 2019, 576(7785). [10] M. S.Dresselhaus, G.Chen, M.Y.Tang et al.New Directions for Low-Dimensional Thermoelectric Materials[J]. Advanced Materials, 2007. [11] J.P.Heremans. Low-dimensional thermoelectricity[J]. Acta Physica Polonica A, 2006, 108(4):609. [12] P.Hyldgaard, G.D.Mahan. Phonon superlattice transport[J]. Physical Review B, 1997, 56(17):10754-10757. [13] A.Balandin, K.L.Wang. Effect of phonon confinement on the thermoelectric figure of merit of quantum wells[J]. Journal of Applied Physics,1998, 84(11):6149-6153. [14] G.Chen, T.Zeng, T.Borca-Tasciuc, et al. Phonon engineering in nanostructures for solid-state energy conversion[J]. Materials Science and Engineering A, 2000, 292(2):155-161. [15] Z.M.Dashevsky, S.Ashmontas, L.Vingelis, et al. The thermoelectric power on p-n junction[C]// Fifteenth International Conference on Thermoelectrics. IEEE, 1996. [16] A.A.Zakhidov, Y.I.Ravich, D.A.Pchenoy-Severin. Thermopower enhancement and optimal ZT in p-n junction arrays[C]// Eighteenth International Conference on Thermoelectrics. IEEE, 1999. [17] Y.I.Ravich, D.A.Pshenai-Severin. Thermoelectric figure of merit of a p-n junction[J]. Semiconductors, 2001, 35(10):1161-1165. [18] M.Wagner, G.Span, T.Grasser. Thermoelectric Power Generation using Large Area Si/SiGe pn-Junctions with varying Ge[J]. Semiconductor Science and Technology, 2007, 22(1):1-2. [19] M.Wagner, G.Span, S.Holzert, et al. Design Optimization of Large Area Si/SiGe Thermoelectric Generators[J]. 2006. [20] D.Y.Fu. Strain and Polarization Induced Band Engineering and The Transport Dynamics of Semiconductors[D]. Nanjing University,2012. [21] J.J.Ebers, J.L.Moll. Large-Signal Behavior of Junction Transistors[J]. Proceedings of the I.R.E, 1954, 42:1761-1772. [22] C.Papadopoulos. Solid-State Electronic Devices. Springer-Verlag New York Inc.

vertical to temperature gradient Bohang Nan, Guiying Xu*, Quanxin Yang and Tao Guo

Beijing Municipal Key Lab of Advanced Energy Materials and Technology, School of Materials Science and Engineering, University of Science and Technology Beijing,

Beijing 100083, China Corresponding authors: [email protected] (G. Xu)

Abstract. We present a model for P-N-P abrupt heterostructures vertical to temperature gradient to

improve the thermoelectric performance. The P-N-P heterostructure is considered as an abrupt bipolar junction transistor due to an externally applied temperature gradient paralleled to depletion layers. Taking Bi2Te3 and Bi0.5Sb1.5Te3 as N-type and P-type thermoelectric materials respectively for example, we achieve the purpose of controlling the Seebeck coefficient and the electrical conductivity independently while amplifying operation power. The calculated results show that the Seebeck coefficient can reach 3312V/K, and the ZTmax values of this model are 45 or 425, which are tens or even hundreds of times greater than those of bulk materials and films.

I. Introduction It is well known that energy issue is imperative for most countries in

the world. Many researchers have searched for novel sustainable and

renewable energy sources in order to alleviate energy consumption needs

and increase utilization efficiency. Thermoelectric materials have

attracted a lot of attention because of their reversible conversion between

heat and electricity.

Thermoelectric performance is quantified by the dimensionless

figure of merit 2 /ZT S T , where S is the Seebeck coefficient, is

the electrical conductivity, T is the absolute temperature and is the

thermal conductivity.[1] Thermal conductivity primarily includes the

lattice thermal conductivity ( L ) and the electronic thermal conductivity

( e ). , 2S is called “power factor” of the thermoelectric material.

However, these parameters are mutually influential, which makes it

difficult to enhance thermoelectric performance. Therefore, most

traditional bulk thermoelectric materials can reach max 1ZT , such as

Bi2Te3, PbTe and SiGe alloys.[2]

Generally speaking, if the commercial thermoelectric materials have

a higher ZT, their conversion efficiency would be higher.[3] And

thermoelectric materials need have ZT values greater than 3 to be

competitive with traditional mechanical equipment.[4]

In order to enhance ZT values, low-dimensional thermoelectric

materials have become the forefront of research since 1990s. Hicks and

Dresselhaus initially presented the concept that low-dimensional

materials could increase their thermoelectric performance after improving

its power factor in 1993.[5] Based on their assumptions, a max 6ZT for

the Bi2Te3 two-dimensional material was obtained. This prediction was

confirmed by many experimental data. The high ZTmax value of 2.4 in

P-type Bi2Te3/Sb2Te3 quantum-well superlattice material was prepared by

Venkatasubramanian et al.[6] Then a greatly enhanced ZTmax value of 3

was obtained in N-type PbSeTe/PbTe quantum-dot superlattice material

by Harman et al.[7] In addition, 1ZT silicon nanowires achieved by

Boukai et al were one hundred times greater than bulk silicon materials.[8]

Hinterleitner et al. prepared Fe2V0.8W0.2Al films by magnetron sputtering,

which reached a maximum ZTmax of 6 around 350-400K.[9]

These enhanced thermoelectric performances mainly originated

from two aspects: (1) the Seebeck coefficient can be improved by

introducing quantum confinement effect;[10,11] (2) the lattice thermal

conductivity can be decreased because phonons are effectively scattered

by interfaces.[12-14] However, there are some questions that hinder the

development of low-dimensional thermoelectric materials. First of all, the

improved ZT values of most low-dimensional thermoelectric materials are

derived from the reduction of the lattice thermal conductivity, rather than

the increase of power factor. Secondly, it is difficult to control S and

independently. Therefore, it is a more common choice to make the

addition of the Seebeck coefficient greater than the reduction of the

electrical conductivity.

In order to solve these questions, we present a model for the P-N-P

heterostructure, which was designed through arranging several P-N

junction thermoelectric materials in a certain structure. In fact, P-N

junctions have been studied a lot and used widely since 1950s. In the late

1990s, P-N junctions were predicted to enhance Seebeck coefficients and

ZT values of thermoelectric materials by Dashevsky,[15] Zakhidov,[16]

Ravich[17] and others. Wagner and Span proposed a new approach that

P-type material and N-type material could be directly connected without

metal electrodes. Meanwhile, a temperature gradient was applied along

this P-N junction, as shown in Figure 1.[18] The measured results

demonstrated that the efficiency of this approach is higher than traditional

P-N junctions.[19] Further research on this approach was carried out by Fu

Deyi et al. Fu Deyi theorized that this approach could increase the

Seebeck coefficient and decrease the electronic thermal conductivity due

to the effect of eddy currents in the P-N junction.[20]

Figure 1. P-N junction with applied temperature gradient

In this work, we propose a P-N-P abrupt heterostructure model

vertical to temperature gradient, and provide the detailed analysis process

along with calculated results. Here, due to the effect of temperature

gradient, the P-N-P heterostructure behaves as a bipolar junction

transistor to achieve power amplification. The collector current is

controlled by the emitter current in a bipolar transistor, while the Seebeck

coefficient is controlled by base-collector interface. The purpose of

independent control with regards to both the Seebeck coefficient and

electrical conductivity is realized. As a result, the ZTmax values can reach

tens or even hundreds of times greater than those of bulk materials and

films.

The paper is organized as follow: In Sec. II we shall describe our

model for P-N-P heterostrctures. In Sec. III we will show and discuss our

calculated results. In Sec. IV we shall conclude.

The scheme that has been adopted with respect to notation is

illustrated by the partial list of symbols shown in Table I. In addition, the

symbol μ has been employed for charge carrier mobility, D for diffusion

constant. Table I. Partial list of symbols used

Symbol meaning

Na, Nd Doping concentration in a P-type material, in a N-type material.

Ex Electric field intensity in an abrupt P-N junction.

xp, xn Depletion layer width near a P-type region, near a N-type region

Electric potential variation in an abrupt P-N junction

r Relative permittivity of the material

0 Vacuum dielectric constant

ni Intrinsic carrier concentration of the material

Vs The Seebeck voltage generated by the temperature gradient.

EC, EV Conduction band minimum of the material, valence band maximum of the material.

EFp, EFn The quasi-Fermi level in a P-type material, in a N-type material.

m* The effective mass of the material.

II. Analytical model for P-N-P heterostructures An analytical model for thermoelectric properties of P-N-P

heterostructure is presented in this section. Under the effect of

temperature gradient, P-N-P heterostructures behave as a bipolar

transistor. A general circuit diagram of a P-N-P heterostructure is shown

in Figure 2, where P-type material (at the left side of this figure) is

considered as an emitter material, N-type material is treated as a base

material, and another P-type material (at the right side of this figure) is

acts as a collector material. In addition, there are depletion layers at the

both of base-emitter interface and at the base-collector interface. The base

width is considered to be the sum of the width of both depletion layers

near N-type region. As a result, the base region can serve as an insulating

layer, in which majority carriers have been depleted. The direction of

temperature gradient is assumed to be parallel to these depletion layers.

Therefore, in the X direction, the Seebeck voltage can be produced due to

the existence of temperature gradient. Meanwhile, the Seebeck voltage

can become an external power supply in the bipolar transistor. We have

biased the emitter forward and the collector in reverse to achieve the

purpose of power amplification. We have also treated the bipolar

transistor as two coupled P-N diodes, according to the Ebers-Moll

model.[21]

In order to simplify this calculation, we have adopted several

assumptions: (1) abrupt P-N junctions; (2) Depletion layer approximation;

(3) Long-length approximation; (4) some assumptions for the bipolar

transistor.

We have divided this bipolar transistor into two coupled P-N

junctions and assumed these P-N junctions are all abrupt junctions, which

means that impurities are uniformly distributed in different regions. For

one abrupt P-N junction, doping levels in P-type material and N-type

material are kept constant when it is away from this junction and will

abruptly change at the junction interfacial region (as in Figure 3b). It is a

consensus that a dN N in the P-type region and d aN N in the N-type

region. As a result physical parameters of the abrupt P-N junction usually

vary in different regions, such as electric field intensity (as in Figure 3c)

electric potential (as in Figure 3d) and doping levels.[22]

Figure 3. (a).An abrupt P-N junction; (b). Doping levels for the abrupt junction; (c). Electric field intensity for the abrupt junction; (d). Electric potential variation for

the abrupt junction.

We have found that the electric field intensity is zero and the electric

potential variation is constant when away from the junction interfacial

region in thermal equilibrium. Therefore, we have divided this P-N

junction into three regions: P-type region, N-type region and depletion

layer, where the depletion layer has an electric potential difference and

other regions are neutral.

(2)Depletion layer approximation

If P-type material and N-type material combine to form a P-N

junction, the majority carriers of two regions will move to the opposite

area due to carrier concentration gradients that exist at the interface. It

results in a depletion layer at the interface when the equilibrium is

reached again.

To solve for the potential barrier biV across the depletion layer, we

have employed the depletion layer approximation. In this assumption,

there are no free electrons and holes in the depletion layer, only impurity

ions ( dN or aN ). Moreover, recombination is completely neglected in the

depletion layer. As a result, the potential barrier biV can be obtained by

solving Possion’s equation:[23]

2 04 / r (1)

2ln d aB bi

(2)

We have also utilized another assumption that the voltage drop will

only appear at the depletion layer if an external voltage (Vs) is applied.

Simultaneously, the potential barrier is independent of the temperature

gradient and external voltage.

Generally, there are different Fermi levels between P-type material

and N-type material. Therefore, the Fermi level can be realigned during

the process of forming a PN junction, resulting in the quasi-Fermi level.

To simplify this analysis, we have adopted the assumption that the

quasi-Fermi level is constant.[24]

In reality, minority carriers of P-type material and N-type material

need to be considered. This is because the recombination of minority

carriers and majority carriers can affect the performance of a P-N

junction. Therefore, the long-length approximation has been employed,

in which the electron and hole diffusion lengths are shorter than the

widths of P-type and N-type regions.[25] In other words, electrons and

holes are recombined completely in the neutral region. The specific

description is shown in Figure 4:

Figure 4: P-N junction in long-length approximation

The quasi-Fermi level ( FnE ) of N-type material is therefore constant

in N-type region and the depletion layer under the same temperature, and

the same applies to P-type material. The quasi-Fermi level is directly

reflected in the dependence of the carrier concentration, resulting in a

convenient calculation for the Seebeck coefficient:

5 2

B F

(3a)

sV S T (3b)

Where 1/ 2r is the phonon scattering parameter, sV is the

Seebeck voltage, and T is the temperature difference.

In this model, we have used Seebeck coefficients of bulk N-type

material and P-type material as the basis for calculating the Seebeck

voltage of the P-N junction.

(4 ) Some assumptions about the bipolar transistor

Although we have divided the bipolar transistor into two P-N

junctions during the analysis process, the expression for volt-ampere

characteristic of the bipolar transistor is still essential when calculating

the overall thermoelectric performance. The suitable expression for

volt-ampere characteristic of the bipolar transistor is not only based on

above assumptions, but also requires some further hypotheses.

In our model, the base width is very thin(around 20nm) and the

recombination of electrons and holes in the base region is neglected so

that the base current is equal to zero, which means that the emitter current

is equal to the collector current. Meanwhile, we have adopted small

injection levels. Therefore, the expression for volt-ampere characteristic

of the bipolar transistor is written as:

/ 1E BpB nB nE pE qV k T E

B nE

W L

where EJ is the emitter current density, B pB pB

k TD q

is the hole

diffusion coefficient of the base material, pB is the minority carrier

mobility of the base material, nBP is the minority carrier concentration of

the base material, BW is the base width, B nE nE

k TD q

is the electron

diffusion coefficient of the emitter material, nE is the minority carrier

mobility of the emitter material, pEN is the minority carrier

concentration of the emitter material, nE nE nEL D is the minority

carrier diffusion length of the emitter material, nE is the relaxation time

of the emitter material, and EV is the emitter voltage.

We have assumed the emitter current is equal to the collector current,

and the current density of both is the same if junction areas of the

base-emitter interface and base-collector interface are identical. Therefore,

E CJ J can be obtained.

Subsequently, the collector voltage and emitter voltage can thus be

determined. We have assumed that the emitter is forward biased and the

collector is reverse biased. In addition, the Seebeck voltage caused by the

temperature gradient is treated as an external power supply for the bipolar

transistor. Moreover, the potential barrier E biV of the base-emitter

interface and the potential barrier C biV of the base-collector interface are

independent of the external voltage. Therefore, the emitter voltage EV

and collector voltage CV can be written as:

E E bi EV V S T (5a)

C C bi CV V S T (5b)

where ES is the Seebeck coefficient of the emitter material, and CS is

the Seebeck coefficient of the collector material.

After determining EV and CV , the depletion layer width ( dCx ) across

the base-collector interface can be written as:

02 r C a

nC d a d

dC nC pCx x x (6c)

where nCx is the depletion layer width near the base region, and

pCx is the depletion layer width near the collector region. And the

depletion layer width across the base-emitter interface ( dE nE pEx x x ) can

also be obtained. Consequently, the base width in Eq.(4) is equal to

nEx + nCx .

The electrical conductivity of the bipolar transistor can be derived

from the emitter current density:

eJ E

base-emitter interface (depletion layer) as the electric field varies linearly

with distance for an abrupt P-N junction.

The Seebeck coefficient of the bipolar transistor can be obtained

based on the collector voltage:

c PNP

VS T

(8)

Finally, the power factor and ZT of the bipolar transistor can also be

obtained:

bipolar transistor can be obtained.

III. Result and Discussion

The model described in this work has been implemented using

MATLAB. Because Bi2Te3 and Sb2Te3 are widely used thermoelectric

semiconductor materials, we applied our model to a

P-Bi0.5Sb1.5Te3/N-Bi2Te3/ P-Bi0.5Sb1.5Te3 heterostructure in order to

evaluate the potentiality of this model. Table II. shows these material

parameters used in the simulation. Table II. Material parameters used for the simulation (Tc=298K Th=323.15K)

Material Parameter

Emitter (P-Bi0.5Sb1.5Te3)

Base (N-Bi2Te3)

Collector (P-Bi0.5Sb1.5Te3)

Eg(eV) 0.18[26] 0.17[27] 0.18 r 260[26] 400[28] 260 m*/m0 1.441[29] 1.4[30] 1.467[29]

n(cm2/V s) 120[31] 1200[17] 120 8000[32] \ 8000[32]

p(cm2/V s) \ 510[17] \ \ 4778.3[33] \

Dn(cm2/s) 3.3446 33.466 3.3446 222.97 \ 222.97

Dp(cm2/s) \ 14.2146 \ \ 133.18 \

doping concentrations for the emitter material, base material and collector

material according to Eq.(3a). In order to obtain the better thermoelectric

performance, we set the range of Seebeck coefficients for these materials

at 220V/K240V/K. Therefore, the scope of doping concentrations

for these materials can subsequently be determined. These results are

derived from experimental data found in previous literature.[29,30]

Figure 5. The relationship between Seebeck coefficients and doping concentrations for (a) the base material, (b) the emitter material, and (c) the collector material

We could estimate the range of doping concentrations for these

materials through calculated results. The range for base material, emitter

material, and collector material is 19 19 32.1 10 2.7 10 / cm ,

19 19 32.2 10 2.8 10 / cm and 19 19 32.2 10 2.8 10 / cm respectively.

2.1 Collector voltage

According to Eq. (5b), the collector voltage is the sum of the

potential barrier of the base-collector interface and the Seebeck voltage.

Moreover, we considered that the collector voltage is a function of the

base doping concentration and collector doping concentration based on

Eq.(2) and Eq.(3a), as shown in Figure 6.

Figure 6. Collector voltage in the P-N-P heterostructure

In order to obtain the maximum output power, the collector voltage

should be at the maximum. We can see that the maximum collector

voltage is 0.1656V when doping concentrations of the base material and

collector material are 19 32.7 10 / cm and 19 32.8 10 / cm , respectively.

Therefore, we can determine the optimal doping concentrations for the

base material and collector material. Subsequently, 11.75nCx nm can be

obtained to calculate the base width .

2.2. Emitter voltage and Emitter current density

After determining the base doping concentration, the emitter voltage

is also derived from Eq.(2), (3a) and (5a). Figure 7 shows the relationship

of the emitter voltage and the emitter doping concentration.

Figure 7. Emitter voltage in the P-N-P heterostructure

We find that the magnitude of the emitter voltage increases as the

emitter doping concentration increases. This finding indicates that the

potential barrier of the base-emitter interface is positively correlated with

the emitter doping concentration and the Seebeck voltage is relatively

small. But we can’t define the optimal doping concentration of the emitter

material just from Figure 8 as the emitter current density is a more

important parameter for the bipolar transistor. As a result, we calculated

the emitter current density based on data presented in Table II. The

relationship between the emitter current density and the emitter doping

concentration under different carrier mobility is shown in Figure 8.

Figure 8. Emitter current density in the P-N-P heterostructure

(a) 2 1 1510p cm V s for the base material, 2 1 1120n cm V s for the

emitter material (b) 2 1 14778p cm V s for the base material,

2 1 18000n cm V s for the emitter material (c) 2 1 1510p cm V s for the

base material, 2 1 18000n cm V s for the emitter material (d)

2 1 14778p cm V s for the base material, 2 1 1120n cm V s for the emitter

material

As it can be seen, there are different emitter current densities under

distinct carrier mobility and the absolute values of emitter current

densities increase with the increase of the emitter doping concentration.

In order to gain the maximum output power, we determined the emitter

current density should be the maximum and also obtained the optimal

emitter doping concentration along with the maximum emitter voltage.

Meanwhile, the depletion layer width ( nE pEx x ) across the base-emitter

interface and the base width ( nEx + nCx ) were determined.

We summarized the maximum emitter current densities under

different conditions in Table III. Table III. The maximum emitter current densities under different carrier mobility

(T=323.15K) Carrier Mobility

It is evident that the maximum emitter current densities remain

almost unchanged when the minority carrier mobility ( p) of the base

material is constant from Table III. This is because the base width is

nanoscale and the electron diffusion length of the emitter material is

micron level. Therefore, we considered that the minority carrier mobility

of the base material is the main factor affecting the maximum emitter

current densities. Moreover, the nanoscale base width results in a large

emitter current density, which increases the output power in the bipolar

transistor.

Because we selected the optimal collector voltage and the maximum

emitter current density, the optimal electrical conductivity and Seebeck

coefficient of the bipolar transistor can be obtained according to Eq.(7)

-(9b). Specific calculation results are shown in Table IV.

Table IV. Electrical conductivities, Seebeck coefficients, power factors and ZT for the P-N-P heterostructure (T=323.15K)

Case Carrier Mobility /cm2/V s

Electrical Conductivity /S/cm

Seebeck Coefficient /V/K

255.9 3312 2807.06 45

2397.7 3312 26301.2 425

256.44 3312 2813 45

2397.7 3312 26301.2 425

The electrical conductivities of all the cases are shown in Table IV.

We can find that these cases have electrical conductivities of about

255.9S/cm, 2397.7S/cm, 256.44S/cm and 2397.7S/cm, respectively. The

magnitude of electrical conductivity of all the cases change with the hole

mobility of base material (N-type Bi2Te3). Compared with N-type Bi2Te3

bulk material ( 1204.5 /S cm )[29] and film ( 2174 /S cm )[34] in previous

literature, electrical conductivities of Case I and Case III are lower than

those of the bulk material and film. Because electrical conductivities are

derived from Eq.(4) and Eq.(7), we consider that the emitter current

density is the main factor affecting electrical conductivities. We can see

that the emitter current density is related to minority carrier

concentrations at the base region and the emitter region in Eq.(4).

Therefore, possible explanation behind the low electrical conductivities

of Case I and Case III is the relatively low minority carrier concentrations

at the base-emitter interface. On the other hand, Case II and Case IV have

almost the same electrical conductivities as films. This is because the

minority carrier mobility of these two cases is larger than those of films

( 210.7 /cm Vs ) in Reference [34]. We believe that the reduction in the

carrier concentration is more than compensated for by the increase in the

carrier mobility.

The Seebeck coefficients of these cases exhibit very large absolute

values, which are 50 times greater than those of films and 15 times

greater than those of bulk materials. We believe that such a large Seebeck

coefficient may be caused by the potential barrier of the depletion layer in

the base-collector interface. In this depletion region, majority carriers can

be depleted completely and the recombination of electrons in N-type

material and holes in P-type material at the cold region under this

temperature gradient can be eliminated. Therefore, the high values of

Seebeck coefficients can be obtained.

So far, we have considered only electrical conductivities and

Seebeck coefficient since it is through these performances that our model

predicts an increase in ZT. However, ZT is also in dependence of the

thermal conductivity . If we assume that the thermal conductivity of the

bipolar transistor is equal to 2W/m K, our calculated results in Table III

imply that the bipolar transistor ZT can be up to dozens of times or even

hundreds of times greater than bulk and film values, giving values

of max 45ZT in Cases I and III and max 425ZT in Cases II and IV at

323.15K.

IV. Summary

In this paper, we present a general model for P-N-P heterostructures.

In our model, P-N-P heterostructures behave as bipolar transistors due to

the setting of temperature gradient. We take an abrupt

P-Bi0.5Sb1.5Te3/N-Bi2Te3/ P-Bi0.5Sb1.5Te3 heterostructure as example to

obtain thermoelectric performance of this model. The electrical

conductivity based on the emitter current density and the Seebeck

coefficient based on the collector voltage for the bipolar transistor were

calculated in order to control the Seebeck coefficient and the electrical

conductivity independently. The conclusion can be obtained as below.

(1) With the optimal doping concentration of 19 32.7 10 / cm ,

19 32.8 10 / cm and 19 32.8 10 / cm for the base material, emitter material and

collector material, respectively, the maximum emitter current density and

the maximum collector voltage under different carrier mobility are 1.892

×1011A/m2 or 1.769×1012A/m2 and 0.1656V. The maxZT values can reach

45 or 425 at 323.15K. Therefore, this model is a useful method to

enhance thermoelectric performances and efficiency.

(2) This P-N-P heterostructure model not only provides a completely

new perspective for research in the thermoelectric field, but also for other

energy conversion mechanisms, such as photovoltaic conversion.

Acknowledgements:

This work was financially supported by The National Key Research

and Development Program of China [Grant No. 2017YFF0204706], by

the Fundamental Research Funds for the Central Universities [Grant No.

FRF-MP-18-005, and FRF-MP-19-005].

B pE

W L

11 32.26 10 /in cm , 2112

6 3 16

, 500BW nm ,

610n s in the base , 75 10p s in the emitter, 2 122.5nBD cm s ,

2 16.5pED cm s , 18pL m ,

2112 5 3

, 8 21.44 10 /EJ A m is shown in the

literature.

We utilize Eq.(A1) to obtain the emitter current density ' EJ based on these data

and compare with EJ .

Therefore, ' 8 21.41 10 /EJ A m is obtained. And the result is very close to

EJ .

Finally, we can conclude that Eq.(4) and Eq.(A1) are all effective for calculating emitter current densities of P-N-P bipolar transistors and N-P-N bipolar transistors.

Reference: [1] G.J. Snyder, E.S. Toberer. Complex thermoelectric materials[J]. Nature Materials, 2008, 7(2):105-114. [2] J.Mao, Z.Liu, Z.Ren. Size effect in thermoelectric materials[J]. Nature, 2016, 1(1). [3] Z.G.Chen, G.Han, L.Yang, L.N.Chen, J.Zou. Nanostructured thermoelectric

materials: Current research and future challenge[J]. Progress in Natural Science Materials International, 2012(6):535-549. [4] C.J.Vineis, A.Shakouri, A.Majumdar, M.G.Kanatzidis. Nanostructured Thermoelectrics: Big Efficiency Gains from Small Features[J]. Advanced Materials, 2010, 22(36):3970-3980. [5] L.D.Hicks, M.S.Dresselhaus.Effect of quantum-well structures on the thermoelectric figure of merit[J]. Physical Review B, 1993, 47 (19):12727-12731. [6] R.Venkatasubramanian, E.Siivola, T.Colpitts, B.O’Quinn.Thin-film thermoelectric devices with high room-temperature figures of merit[J]. Nature, 2001, 413: 597-602. [7] T.C.Harman, M.P.Walsh, B.E.Laforge, G.W.Turner. Nanostructured thermoelectric materials[J]. Journal of Electronic Materials, 2005, 34(5):L19-L22. [8] A.I.Boukai, Y.Bunimovich, J.Tahir-Kheli, et al. Silicon nanowires as efficient thermoelectric materials[J]. Nature, 2008, 451(7175):168-171 [9] B.Hinterleitner B, I.Knapp, M.Poneder, et al. Thermoelectric performance of a metastable thin-film Heusler alloy[J]. Nature, 2019, 576(7785). [10] M. S.Dresselhaus, G.Chen, M.Y.Tang et al.New Directions for Low-Dimensional Thermoelectric Materials[J]. Advanced Materials, 2007. [11] J.P.Heremans. Low-dimensional thermoelectricity[J]. Acta Physica Polonica A, 2006, 108(4):609. [12] P.Hyldgaard, G.D.Mahan. Phonon superlattice transport[J]. Physical Review B, 1997, 56(17):10754-10757. [13] A.Balandin, K.L.Wang. Effect of phonon confinement on the thermoelectric figure of merit of quantum wells[J]. Journal of Applied Physics,1998, 84(11):6149-6153. [14] G.Chen, T.Zeng, T.Borca-Tasciuc, et al. Phonon engineering in nanostructures for solid-state energy conversion[J]. Materials Science and Engineering A, 2000, 292(2):155-161. [15] Z.M.Dashevsky, S.Ashmontas, L.Vingelis, et al. The thermoelectric power on p-n junction[C]// Fifteenth International Conference on Thermoelectrics. IEEE, 1996. [16] A.A.Zakhidov, Y.I.Ravich, D.A.Pchenoy-Severin. Thermopower enhancement and optimal ZT in p-n junction arrays[C]// Eighteenth International Conference on Thermoelectrics. IEEE, 1999. [17] Y.I.Ravich, D.A.Pshenai-Severin. Thermoelectric figure of merit of a p-n junction[J]. Semiconductors, 2001, 35(10):1161-1165. [18] M.Wagner, G.Span, T.Grasser. Thermoelectric Power Generation using Large Area Si/SiGe pn-Junctions with varying Ge[J]. Semiconductor Science and Technology, 2007, 22(1):1-2. [19] M.Wagner, G.Span, S.Holzert, et al. Design Optimization of Large Area Si/SiGe Thermoelectric Generators[J]. 2006. [20] D.Y.Fu. Strain and Polarization Induced Band Engineering and The Transport Dynamics of Semiconductors[D]. Nanjing University,2012. [21] J.J.Ebers, J.L.Moll. Large-Signal Behavior of Junction Transistors[J]. Proceedings of the I.R.E, 1954, 42:1761-1772. [22] C.Papadopoulos. Solid-State Electronic Devices. Springer-Verlag New York Inc.